Science and Technology of Advanced Materials, 2017 VOL. 18, NO. 1, 351–363 https://doi.org/10.1080/14686996.2017.1316422
Magnetization reversal in YIG/GGG(111) nanoheterostructures grown by laser molecular beam epitaxy Boris B. Krichevtsova , Sergei V. Gasteva, Sergey M. Suturina, Vladimir V. Fedorova, Alexander M. Korovina, Viktor E. Bursiana, Alexander G. Banshchikova, Mikhail P. Volkova, Masao Tabuchib and Nikolai S. Sokolova a
Divisions of Solid State Physics and Physics of Dielectrics and Semiconductors, Ioffe Physical-Technical Institute of Russian Academy of Sciences, St Petersburg, Russia b Synchrotron Radiation Research Center, Nagoya University, Nagoya, Japan
Thin (4–20 nm) yttrium iron garnet (Y3Fe5O12, YIG) layers have been grown on gadolinium gallium garnet (Gd3Ga5O12, GGG) 111-oriented substrates by laser molecular beam epitaxy in 700–1000 °C growth temperature range. The layers were found to have atomically flat step-andterrace surface morphology with step height of 1.8 Å characteristic for YIG(111) surface. As the growth temperature is increased from 700 to 1000 °C the terraces become wider and the growth gradually changes from layer by layer to step-flow regime. Crystal structure studied by electron and X-ray diffraction showed that YIG lattice is co-oriented and laterally pseudomorphic to GGG with small rhombohedral distortion present perpendicular to the surface. Measurements of magnetic moment, magneto-optical polar and longitudinal Kerr effect (MOKE), and X-ray magnetic circular dichroism (XMCD) were used for study of magnetization reversal for different orientations of magnetic field. These methods and ferromagnetic resonance studies have shown that in zero magnetic field magnetization lies in the film plane due to both shape and induced anisotropies. Vectorial MOKE studies have revealed the presence of an in-plane easy magnetization axis. In-plane magnetization reversal was shown to occur through combination of reversible rotation and abrupt irreversible magnetization jump, the latter caused by domain wall nucleation and propagation. The field at which the flip takes place depends on the angle between the applied magnetic field and the easy magnetization axis and can be described by the modified Stoner–Wohlfarth model taking into account magnetic field dependence of the domain wall energy. Magnetization curves of individual tetrahedral and octahedral magnetic Fe3+ sublattices were studied by XMCD.
1. Introduction Yttrium iron garnet (YIG) is a model object for study of magnetism in crystals. Its structural, electrical, magnetic, optical and acoustic properties have been intensively discussed since the middle of the last century [e.g.1,2]. The interest in YIG is related to its unique
Received 7 November 2016 Revised 1 April 2017 Accepted 4 April 2017 KEYWORDS
YIG nanolayers; magnetization process; magnetic anisotropy; laser MBE; XMCD; AFM; XRD; MOKE CLASSIFICATION
40 Optical, magnetic and electronic device materials; 102 Porous / Nanoporous / Nanostructured materials; 203 Magnetics / Spintronics / Superconductors; 306 Thin film / Coatings
physical properties such as high optical transparency in a wide range of wavelengths, high Curie temperature, ultra-low spin wave and acoustic wave damping, and strong magneto-optical effects. In the 1970–1980s much attention was paid to fabrication of heterostructures with garnet layers because of the development of
CONTACT Boris B. Krichevtsov [email protected]
Supplemental data for this article can be accessed here. [https://doi.org/10.1080/14686996.2017.1316422] © 2017 The Author(s). Published by National Institute for Materials Science in partnership with Taylor & Francis. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.
Sci. Technol. Adv. Mater. 18 (2017) 352B. B. KRICHEVTSOV et al.
new magneto-optic [3,4] and microwave  devices as well as applications utilizing cylindrical domain control for data storage and processing [6–8]. Garnet films of micrometer thickness were routinely grown by liquid phase epitaxy. Extensive studies of static, dynamic, magnetic and magneto-optical properties of such films have been carried out [1,3,4,9]. It has been shown that magnetic anisotropy (in-plane, out of plane, rhombic) in thick YIG based heterostructures can be tailored by tuning the film/substrate composition and lattice parameters. The study of magnetization reversal and domain structure in garnet films showed that structurally and magnetically the interface differs from the bulk of the film. Although from crystallographic and magnetic points of view YIG and gadolinium gallium garnet (GGG) are centrosymmetric, near the interface the center of symmetry is lost, giving rise to optical second harmonic generation of crystallographic  and magnetic  types as well as to linear magnetoelectric effect [12,13]. The interest in YIG nanostructures, their fabrication and properties, has developed only recently, as new research fields, such as oxide spintronics, magnonics [14–16] and spin caloritronics , have branched off owing to developments in spintronics. Ultrathin magnetic insulating layers (e.g. YIG) may find applications in spintronics for data transmission in the form of spin wave packets . This approach may provide certain advantages over spin-polarized electron currents or spin currents that can be induced in conductive media. Understanding YIG growth is also of great interest in studies of YIG/(Pt, Ta) metal-insulator heterostructures [19–25] for spin pumping and spin transfer, as well as for YIG growth on topological insulators . The growth of thin high-quality epitaxial YIG layers has become possible upon development of laser molecular beam epitaxy (MBE). A number of recent works have addressed the growth of nanometer sized YIG layers on gallium gadolinium garnet GGG substrate. Investigations into structural, magneto-optical, static and dynamic magnetic properties of such layers have been reported [27–37]. It has been shown that magnetization in YIG layers is lower than in bulk crystals because the interface and surface regions are rich with defects and deficient in 3d bonds. Besides this, magnetic ordering different from bulk was observed near the interface . The interfaces are supposed to be responsible for additional spin wave damping channels through magnon scattering on interface defects and through two-magnon decay. Nevertheless spin wave damping in such nanostructures may be low enough and comparable to values obtained for YIG single crystals [35–37], being a prerequisite for fabrication of novel effective spin wave devices. It must be noted that up to now more attention has been paid to static and dynamic magnetic properties than to the magnetization reversal process. The latter is an important characteristic of a magnetic material and
bears information not only about the magnetic interaction defining the change in magnetic state in applied magnetic field, but also about the structural quality of material. In YIG/GGG(111) structures grown by pulsed laser deposition the in-plane magnetization reversal is characterized by low coercivity (Hc ~ 1 Oe) hysteresis that may be accompanied by reversible magnetization rotation . To the best of our knowledge this process has been studied only scarcely. The aim of the present work is to grow YIG layers by laser MBE, to characterize their structural properties and to study mechanisms responsible for magnetization reversal in the in-plane and out-of-plane magnetic fields. The grown YIG/GGG(111) samples have been characterized by synchrotron X-ray diffraction (XRD), high-energy electron diffraction (RHEED) and atomic force microscopy (AFM). The magnetization reversal has been investigated using magneto-optical methods in X-ray and visible light range and by vibrating sample magnetometry (VSM). Magnetization dynamics was studied using ferromagnetic resonance spectroscopy.
2. Experimental details YIG/GGG (111) heterostructures were grown by laser molecular beam epitaxy. The polished (111)-cut GGG substrates were annealed prior to growth for 3 h at 1000 °C in 0.5 mbar of oxygen to improve surface morphology. A stoichiometric Y3Fe5O12 target was ablated by 1 Hz × 10 ns pulses of KrF excimer laser (λ ≈ 248 nm) at a fluence of ~3.1 J cm–2. YIG layers were grown in 0.02 mbar of oxygen at substrate temperature of 700– 1000 °C. The indicated temperatures were measured inside the stainless steel sample holder to which the sample was attached by silver paste glue. More than 20 YIG/GGG samples have been fabricated to understand the influence of growth parameters on YIG growth. In what follows we present data proved to be typical for particular growth regimes. Crystal structure of YIG layers was investigated in situ by enhanced RHEED 3D mapping technique that allows measuring and visualizing three dimensional intensity distribution within a large reciprocal space volume, building arbitrary reciprocal space cross-sections/projections and performing comparison to model reciprocal lattices . The 3D mapping was carried out by collecting series of RHEED patterns during sample rotation around the surface normal. More precise information on the crystal structure was obtained ex situ during synchrotron measurements at BL3A X-ray diffraction beamline (Photon Factory, Tsukuba, Japan). Intensity profiles along YIG/GGG (111) crystal truncation rods (CTR) were measured by point silicon drift detector as well as by applying the 3D mapping approach similar to the one described above. Dense series of XRD patterns were recorded with Pilatus 100 K detector sweeping the reciprocal space volume containing GGG and YIG CTR
Sci. Technol. Adv. Mater. 18 (2017) 353B. B. KRICHEVTSOV et al.
Figure 1. XMCD experiment geometries (a, b). MOKE experiment geometries: LMOKE|| (c) and LMOKE⊥ (d) for measuring in-plane magnetization components, PMOKE (e) for measuring out-of-plane magnetization components.
diffuse scattering around Bragg reflections and the background that has to be taken into account for accurate CTR modeling. Surface morphology of the grown layers was characterized by NT-MDT atomic force microscope in semi-contact mode. X-ray absorption (XAS) and X-ray magnetic circular dichroism (XMCD) measurements at Fe L edge were performed at BL16 beamline of Photon Factory synchrotron (Tsukuba, Japan). The measurements were carried out in surface sensitive total electron yield (TEY) mode keeping the sample biased at –12 V to decrease the influence of magnetic field on the measured electron current. XMCD measurements were carried out in magnetic fields of up to 12 kOe applied parallel to the beam direction. The beam was incident at 30 or 90° to the surface (Figure 1(a) and 1(b)). The TEY spectra were normalized to incident beam intensity and to the pre-edge intensity. The XMCD asymmetry signal at fixed energy and magnetic field was derived from the difference in absorption measured in σ+ and σ– circular polarized light (degree of circular polarization 96%). To increase sensitivity the incident light polarization was modulated at 10 Hz. The in-plane magnetization curves were studied in the Quantum Design PPMS-9 system (Quantum Design Inc., San Diego, CA, USA) at room temperature. The net magnetic moment was calculated from magnetization taking into account the film thickness derived from RHEED and XRD data. Complementary to this, magnetization curves have been measured using vectorial magneto optical Kerr-effect set-up operating at λ = 405 nm. To gain sensitivity the incident light polarization was modulated with a quartz photo-elastic modulator (50 kHz) or a Faraday cell (400 Hz). In-plane magnetization components parallel (M||) and perpendicular (M⊥)
to the applied in-plane magnetic field were measured using longitudinal magneto-optical Kerr effect by orienting the light incident plane parallel (LMOKE||) and perpendicular (LMOKE⊥) to the magnetic field direction (Figure 1(c) and 1(d)). In this set-up the light was incident at 45° to the surface in S-polarization geometry. The out-of-plane magnetization curves in magnetic fields of up to 20 kOe (4 kOe) were investigated by measured polar MOKE (PMOKE) effect at 87° (45°) incidence (Figure 1(e)). The beam was focused to a small spot 0.3 mm in diameter to allow precise area selective studies. Ferromagnetic resonance (FMR) spectra were measured on an electron paramagnetic resonance spectrometer at 9.41 GHz in magnetic field of up to 10 kOe applied in-plane or out-of-plane.
3. Surface morphology and lattice structure 3.1. Atomic force microscopy The role of GGG substrate annealing prior to YIG growth becomes evident from analysis of AFM surface morphology images measured before and after 1000 °C annealing in oxygen (Figure 2(a) and 2(b)). The original substrate surface is rough (rms > 2.5 Å) showing traces of polishing. In contrast to this, the annealed surface shows atomically flat terraces separated by monoatomic steps (rms